#------------------------------------------------------------------------------
#$Date: 2020-03-05 01:43:20 +0200 (Thu, 05 Mar 2020) $
#$Revision: 248863 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/13/43/4134337.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4134337
loop_
_publ_author_name
'Guo, Shu'
'Zhong, Ruidan'
'Wang, Wei'
'Tao, Jing'
'Ni, Danrui'
'Cava, Robert J.'
_publ_section_title
;
 K₃Ir₂O₆ and
 K<sub>16.3</sub>Ir₈O₃₀, Low dimensional Iridates
 with Infinite IrO₆ Chains.
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_paper_doi               10.1021/jacs.0c00849
_journal_year                    2020
_chemical_formula_moiety         '0.17(Ir12 K18 O36)'
_chemical_formula_sum            'Ir2 K3 O6'
_chemical_formula_weight         597.70
_space_group_crystal_system      trigonal
_space_group_IT_number           148
_space_group_name_Hall           '-R 3'
_space_group_name_H-M_alt        'R -3 :H'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_date             2020-01-20
_audit_creation_method
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            6
_cell_length_a                   10.8202(6)
_cell_length_b                   10.8202(6)
_cell_length_c                   10.5416(6)
_cell_measurement_reflns_used    3273
_cell_measurement_temperature    290
_cell_measurement_theta_max      33.22
_cell_measurement_theta_min      3.77
_cell_volume                     1068.83(10)
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'XL (Sheldrick, 2008)'
_computing_structure_solution    'XS (Sheldrick, 2008)'
_diffrn_ambient_temperature      290
_diffrn_detector                 'Bruker APEX2 area detector'
_diffrn_detector_area_resol_mean 7.9
_diffrn_detector_type            'CCD area detector'
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device       'three-circle diffractometer'
_diffrn_measurement_device_type  'Bruker SMART APEX2 area detector'
_diffrn_measurement_method       'ω and φ scans'
_diffrn_radiation_monochromator  'mirror optics'
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0315
_diffrn_reflns_av_unetI/netI     0.0174
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            8925
_diffrn_reflns_theta_full        33.22
_diffrn_reflns_theta_max         33.22
_diffrn_reflns_theta_min         2.91
_diffrn_source                   'microfocus sealed X-ray tube'
_diffrn_source_type              'Incoatec I\ms'
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    39.040
_exptl_absorpt_correction_T_max  0.7465
_exptl_absorpt_correction_T_min  0.2991
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
SADABS-2016/2 (Bruker,2016/2) was used for absorption correction.
wR2(int) was 0.1281 before and 0.0245 after correction.
The Ratio of minimum to maximum transmission is 0.4007.
The λ/2 correction factor is Not present.
;
_exptl_crystal_colour            black
_exptl_crystal_colour_primary    black
_exptl_crystal_density_diffrn    5.572
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       needle
_exptl_crystal_F_000             1554
_exptl_crystal_size_max          0.137
_exptl_crystal_size_mid          0.064
_exptl_crystal_size_min          0.036
_refine_diff_density_max         1.032
_refine_diff_density_min         -1.465
_refine_diff_density_rms         0.336
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.083
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     36
_refine_ls_number_reflns         915
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.083
_refine_ls_R_factor_all          0.0423
_refine_ls_R_factor_gt           0.0195
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0160P)²+2.4414P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0357
_refine_ls_wR_factor_ref         0.0410
_reflns_number_gt                622
_reflns_number_total             915
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ja0c00849_si_003.cif
_cod_data_source_block           190914_ki_800_290_1_0m
_cod_original_sg_symbol_H-M      'R -3'
_cod_database_code               4134337
_olex2_refinement_description
;
1. Twinned data refinement
 Scales: 0.605(3)
 0.395(3)
;
_olex2_submission_special_instructions 'No special instructions were received'
loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 'x, y, z'
2 '-y, x-y, z'
3 '-x+y, -x, z'
4 'x+2/3, y+1/3, z+1/3'
5 '-y+2/3, x-y+1/3, z+1/3'
6 '-x+y+2/3, -x+1/3, z+1/3'
7 'x+1/3, y+2/3, z+2/3'
8 '-y+1/3, x-y+2/3, z+2/3'
9 '-x+y+1/3, -x+2/3, z+2/3'
10 '-x, -y, -z'
11 'y, -x+y, -z'
12 'x-y, x, -z'
13 '-x+2/3, -y+1/3, -z+1/3'
14 'y+2/3, -x+y+1/3, -z+1/3'
15 'x-y+2/3, x+1/3, -z+1/3'
16 '-x+1/3, -y+2/3, -z+2/3'
17 'y+1/3, -x+y+2/3, -z+2/3'
18 'x-y+1/3, x+2/3, -z+2/3'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_calc_flag
_atom_site_disorder_assembly
_atom_site_disorder_group
_atom_site_site_symmetry_order
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
Ir1 Ir 0.0000 0.0000 0.0000 0.00639(10) Uani 1 d . . 6 S T P
Ir2 Ir 0.0000 0.0000 0.5000 0.00651(10) Uani 1 d . . 6 S T P
Ir3 Ir 0.0000 0.0000 0.25099(3) 0.00631(7) Uani 1 d . . 3 S T P
K1 K 0.03638(13) 0.30896(12) 0.17585(14) 0.0181(2) Uani 1 d . . 1 . . .
O1 O 0.1486(3) 0.1284(3) 0.1248(3) 0.0102(7) Uani 1 d . . 1 . . .
O2 O 0.0270(4) 0.1514(3) 0.3760(3) 0.0105(7) Uani 1 d . . 1 . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ir Ir -1.4442 7.9887 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Ir3 Ir1 Ir3 180.0 10 . ?
Ir3 Ir1 K1 59.64(2) 10 10 ?
Ir3 Ir1 K1 120.36(2) . 12 ?
Ir3 Ir1 K1 59.64(2) . 3 ?
Ir3 Ir1 K1 120.36(2) . 10 ?
Ir3 Ir1 K1 120.36(2) 10 3 ?
Ir3 Ir1 K1 120.36(2) 10 . ?
Ir3 Ir1 K1 59.64(2) . . ?
Ir3 Ir1 K1 59.64(2) 10 12 ?
K1 Ir1 K1 96.71(3) 10 12 ?
K1 Ir1 K1 96.71(3) . 3 ?
K1 Ir1 K1 83.29(3) 10 3 ?
K1 Ir1 K1 83.29(3) . 12 ?
K1 Ir1 K1 180.00(5) 10 . ?
K1 Ir1 K1 180.00(6) 12 3 ?
O1 Ir1 Ir3 131.05(9) 2 10 ?
O1 Ir1 Ir3 48.95(9) 2 . ?
O1 Ir1 Ir3 48.95(9) 3 . ?
O1 Ir1 Ir3 48.95(9) 11 10 ?
O1 Ir1 Ir3 131.05(9) 12 . ?
O1 Ir1 Ir3 131.05(9) . 10 ?
O1 Ir1 Ir3 131.05(9) 10 . ?
O1 Ir1 Ir3 48.95(9) 12 10 ?
O1 Ir1 Ir3 131.05(9) 11 . ?
O1 Ir1 Ir3 131.05(9) 3 10 ?
O1 Ir1 Ir3 48.95(9) . . ?
O1 Ir1 Ir3 48.95(9) 10 10 ?
O1 Ir1 K1 71.42(10) 3 10 ?
O1 Ir1 K1 130.35(10) 12 3 ?
O1 Ir1 K1 48.16(10) . 3 ?
O1 Ir1 K1 131.84(10) 2 10 ?
O1 Ir1 K1 108.58(10) 12 10 ?
O1 Ir1 K1 48.16(10) 11 10 ?
O1 Ir1 K1 108.58(10) 2 3 ?
O1 Ir1 K1 49.65(10) . . ?
O1 Ir1 K1 108.58(10) 3 . ?
O1 Ir1 K1 130.35(10) . 10 ?
O1 Ir1 K1 71.42(10) 12 . ?
O1 Ir1 K1 108.58(10) 11 12 ?
O1 Ir1 K1 131.84(10) 10 3 ?
O1 Ir1 K1 49.65(10) 12 12 ?
O1 Ir1 K1 71.42(10) 11 3 ?
O1 Ir1 K1 130.35(10) 3 12 ?
O1 Ir1 K1 49.65(10) 3 3 ?
O1 Ir1 K1 130.35(10) 10 . ?
O1 Ir1 K1 48.16(10) 2 . ?
O1 Ir1 K1 48.16(10) 10 12 ?
O1 Ir1 K1 49.65(10) 10 10 ?
O1 Ir1 K1 71.42(10) 2 12 ?
O1 Ir1 K1 131.84(10) 11 . ?
O1 Ir1 K1 131.84(10) . 12 ?
O1 Ir1 O1 180.00(14) 2 11 ?
O1 Ir1 O1 98.46(14) 11 3 ?
O1 Ir1 O1 98.46(14) . 11 ?
O1 Ir1 O1 98.46(14) . 12 ?
O1 Ir1 O1 180.0(2) . 10 ?
O1 Ir1 O1 81.54(14) 10 12 ?
O1 Ir1 O1 81.54(14) 2 3 ?
O1 Ir1 O1 98.46(14) 2 12 ?
O1 Ir1 O1 180.0(2) 12 3 ?
O1 Ir1 O1 81.54(14) 11 12 ?
O1 Ir1 O1 98.46(14) 10 2 ?
O1 Ir1 O1 81.54(14) . 3 ?
O1 Ir1 O1 81.54(14) 10 11 ?
O1 Ir1 O1 98.46(14) 10 3 ?
O1 Ir1 O1 81.54(14) . 2 ?
Ir3 Ir2 Ir3 180.0 10_556 . ?
Ir3 Ir2 K1 91.55(2) 10_556 16 ?
Ir3 Ir2 K1 88.45(2) 10_556 4_445 ?
Ir3 Ir2 K1 88.45(2) 10_556 5 ?
Ir3 Ir2 K1 88.45(2) . 16 ?
Ir3 Ir2 K1 91.55(2) 10_556 17_445 ?
Ir3 Ir2 K1 91.55(2) . 4_445 ?
Ir3 Ir2 K1 88.45(2) . 17_445 ?
Ir3 Ir2 K1 91.55(2) . 5 ?
K1 Ir2 K1 60.071(2) 17_445 4_445 ?
K1 Ir2 K1 119.929(2) 5 4_445 ?
K1 Ir2 K1 119.929(2) 17_445 16 ?
K1 Ir2 K1 180.0 16 4_445 ?
K1 Ir2 K1 60.071(2) 5 16 ?
K1 Ir2 K1 180.0 5 17_445 ?
O2 Ir2 Ir3 49.18(9) 10_556 10_556 ?
O2 Ir2 Ir3 130.82(9) 10_556 . ?
O2 Ir2 Ir3 130.82(9) 11_556 . ?
O2 Ir2 Ir3 49.18(9) 3 . ?
O2 Ir2 Ir3 130.82(9) 2 10_556 ?
O2 Ir2 Ir3 130.82(9) . 10_556 ?
O2 Ir2 Ir3 49.18(9) 2 . ?
O2 Ir2 Ir3 130.82(9) 12_556 . ?
O2 Ir2 Ir3 130.82(9) 3 10_556 ?
O2 Ir2 Ir3 49.18(9) 11_556 10_556 ?
O2 Ir2 Ir3 49.18(9) 12_556 10_556 ?
O2 Ir2 Ir3 49.18(9) . . ?
O2 Ir2 K1 54.09(9) 11_556 5 ?
O2 Ir2 K1 99.49(10) 12_556 16 ?
O2 Ir2 K1 45.69(10) 11_556 16 ?
O2 Ir2 K1 125.91(9) 2 5 ?
O2 Ir2 K1 54.09(9) 10_556 4_445 ?
O2 Ir2 K1 45.69(10) 3 5 ?
O2 Ir2 K1 125.91(9) 10_556 16 ?
O2 Ir2 K1 80.51(10) 10_556 5 ?
O2 Ir2 K1 45.69(10) 2 4_445 ?
O2 Ir2 K1 99.49(10) . 5 ?
O2 Ir2 K1 80.51(10) 12_556 4_445 ?
O2 Ir2 K1 134.31(10) 12_556 5 ?
O2 Ir2 K1 134.31(10) 2 16 ?
O2 Ir2 K1 125.91(9) 11_556 17_445 ?
O2 Ir2 K1 54.09(9) . 16 ?
O2 Ir2 K1 54.09(9) 2 17_445 ?
O2 Ir2 K1 134.31(10) 11_556 4_445 ?
O2 Ir2 K1 134.31(10) 3 17_445 ?
O2 Ir2 K1 99.49(10) 3 4_445 ?
O2 Ir2 K1 99.49(10) 10_556 17_445 ?
O2 Ir2 K1 125.91(9) . 4_445 ?
O2 Ir2 K1 80.51(10) . 17_445 ?
O2 Ir2 K1 45.69(10) 12_556 17_445 ?
O2 Ir2 K1 80.51(10) 3 16 ?
O2 Ir2 O2 81.89(14) 2 3 ?
O2 Ir2 O2 98.11(14) . 12_556 ?
O2 Ir2 O2 180.0 10_556 . ?
O2 Ir2 O2 81.89(14) 11_556 10_556 ?
O2 Ir2 O2 81.89(14) 2 . ?
O2 Ir2 O2 98.11(14) 2 10_556 ?
O2 Ir2 O2 180.00(19) 11_556 2 ?
O2 Ir2 O2 98.11(14) 3 10_556 ?
O2 Ir2 O2 98.11(14) 11_556 . ?
O2 Ir2 O2 98.11(14) 11_556 3 ?
O2 Ir2 O2 81.89(14) 3 . ?
O2 Ir2 O2 98.11(14) 2 12_556 ?
O2 Ir2 O2 81.89(14) 11_556 12_556 ?
O2 Ir2 O2 180.0 3 12_556 ?
O2 Ir2 O2 81.89(14) 10_556 12_556 ?
Ir1 Ir3 K1 75.95(3) . 2 ?
Ir1 Ir3 K1 75.95(3) . 3 ?
Ir1 Ir3 K1 75.95(3) . . ?
Ir2 Ir3 Ir1 180.0 . . ?
Ir2 Ir3 K1 104.05(3) . 3 ?
Ir2 Ir3 K1 104.05(3) . . ?
Ir2 Ir3 K1 104.05(3) . 2 ?
K1 Ir3 K1 114.30(2) 2 3 ?
K1 Ir3 K1 114.30(2) . 3 ?
K1 Ir3 K1 114.30(2) 2 . ?
O1 Ir3 Ir1 48.63(9) 3 . ?
O1 Ir3 Ir1 48.63(9) 2 . ?
O1 Ir3 Ir1 48.63(9) . . ?
O1 Ir3 Ir2 131.37(9) . . ?
O1 Ir3 Ir2 131.37(9) 3 . ?
O1 Ir3 Ir2 131.37(9) 2 . ?
O1 Ir3 K1 124.57(10) 3 . ?
O1 Ir3 K1 124.57(10) 2 3 ?
O1 Ir3 K1 57.63(10) . 3 ?
O1 Ir3 K1 59.11(9) . . ?
O1 Ir3 K1 59.11(9) 3 3 ?
O1 Ir3 K1 59.11(10) 2 2 ?
O1 Ir3 K1 124.57(10) . 2 ?
O1 Ir3 K1 57.63(10) 3 2 ?
O1 Ir3 K1 57.63(10) 2 . ?
O1 Ir3 O1 81.07(14) 3 . ?
O1 Ir3 O1 81.07(14) 2 . ?
O1 Ir3 O1 81.07(14) 2 3 ?
O2 Ir3 Ir1 131.05(9) . . ?
O2 Ir3 Ir1 131.05(9) 3 . ?
O2 Ir3 Ir1 131.05(9) 2 . ?
O2 Ir3 Ir2 48.95(9) . . ?
O2 Ir3 Ir2 48.95(9) 2 . ?
O2 Ir3 Ir2 48.95(9) 3 . ?
O2 Ir3 K1 55.19(10) 2 2 ?
O2 Ir3 K1 124.25(10) 3 . ?
O2 Ir3 K1 55.19(10) 3 3 ?
O2 Ir3 K1 55.19(10) . . ?
O2 Ir3 K1 119.10(10) . 3 ?
O2 Ir3 K1 124.25(10) 2 3 ?
O2 Ir3 K1 119.10(10) 2 . ?
O2 Ir3 K1 124.25(10) . 2 ?
O2 Ir3 K1 119.10(10) 3 2 ?
O2 Ir3 O1 99.92(13) 2 3 ?
O2 Ir3 O1 97.48(13) 3 3 ?
O2 Ir3 O1 97.48(13) 2 2 ?
O2 Ir3 O1 99.92(13) 3 . ?
O2 Ir3 O1 178.12(12) 2 . ?
O2 Ir3 O1 178.12(12) . 3 ?
O2 Ir3 O1 99.92(13) . 2 ?
O2 Ir3 O1 97.48(13) . . ?
O2 Ir3 O1 178.12(12) 3 2 ?
O2 Ir3 O2 81.56(14) . 2 ?
O2 Ir3 O2 81.56(14) 3 2 ?
O2 Ir3 O2 81.56(14) . 3 ?
Ir2 K1 K1 98.68(4) 7_554 6_455 ?
Ir2 K1 K1 80.07(4) 7_554 8_554 ?
Ir2 K1 K1 59.963(1) 7_554 15 ?
Ir2 K1 K1 59.965(1) 7_554 14_455 ?
Ir3 K1 Ir2 134.11(4) . 7_554 ?
Ir3 K1 K1 76.56(4) . 15 ?
Ir3 K1 K1 81.07(4) . 6_455 ?
Ir3 K1 K1 161.33(5) . 14_455 ?
Ir3 K1 K1 119.40(4) . 8_554 ?
K1 K1 K1 108.84(6) 15 6_455 ?
K1 K1 K1 84.58(6) 14_455 6_455 ?
K1 K1 K1 71.16(6) 14_455 8_554 ?
K1 K1 K1 152.77(5) 8_554 6_455 ?
K1 K1 K1 94.18(5) 15 8_554 ?
K1 K1 K1 119.712(9) 15 14_455 ?
O1 K1 Ir2 159.45(8) 2 7_554 ?
O1 K1 Ir2 110.04(8) 14_455 7_554 ?
O1 K1 Ir2 106.17(7) . 7_554 ?
O1 K1 Ir3 37.89(7) 2 . ?
O1 K1 Ir3 37.77(7) . . ?
O1 K1 Ir3 111.72(9) 14_455 . ?
O1 K1 K1 102.89(8) 2 15 ?
O1 K1 K1 134.15(8) 2 14_455 ?
O1 K1 K1 97.78(8) 2 6_455 ?
O1 K1 K1 47.06(7) . 15 ?
O1 K1 K1 90.78(7) 2 8_554 ?
O1 K1 K1 160.74(9) . 14_455 ?
O1 K1 K1 112.03(8) . 6_455 ?
O1 K1 K1 87.78(9) 14_455 8_554 ?
O1 K1 K1 169.14(9) 14_455 15 ?
O1 K1 K1 51.00(8) 14_455 14_455 ?
O1 K1 K1 66.91(9) 14_455 6_455 ?
O1 K1 K1 94.19(8) . 8_554 ?
O1 K1 O1 87.75(11) 14_455 2 ?
O1 K1 O1 55.83(13) 2 . ?
O1 K1 O1 143.51(11) 14_455 . ?
O1 K1 O2 100.60(11) 14_455 . ?
O1 K1 O2 89.78(10) . 16 ?
O1 K1 O2 141.29(10) 2 16 ?
O1 K1 O2 123.45(11) 14_455 16 ?
O2 K1 Ir2 115.82(8) . 7_554 ?
O2 K1 Ir2 33.84(6) 16 7_554 ?
O2 K1 Ir2 33.14(7) 8_554 7_554 ?
O2 K1 Ir3 37.89(7) . . ?
O2 K1 Ir3 104.23(7) 16 . ?
O2 K1 Ir3 145.58(9) 8_554 . ?
O2 K1 K1 130.18(10) . 14_455 ?
O2 K1 K1 81.57(9) . 15 ?
O2 K1 K1 46.01(7) 16 15 ?
O2 K1 K1 53.08(7) 8_554 14_455 ?
O2 K1 K1 77.73(7) 16 6_455 ?
O2 K1 K1 73.80(8) 8_554 15 ?
O2 K1 K1 157.29(9) . 8_554 ?
O2 K1 K1 110.83(8) 16 8_554 ?
O2 K1 K1 45.72(8) . 6_455 ?
O2 K1 K1 125.05(9) 8_554 6_455 ?
O2 K1 K1 47.20(8) 8_554 8_554 ?
O2 K1 K1 84.18(7) 16 14_455 ?
O2 K1 O1 100.11(10) 8_554 14_455 ?
O2 K1 O1 136.22(10) 8_554 2 ?
O2 K1 O1 66.56(11) . . ?
O2 K1 O1 68.72(10) . 2 ?
O2 K1 O1 107.82(10) 8_554 . ?
O2 K1 O2 82.22(11) . 16 ?
O2 K1 O2 148.03(9) 8_554 . ?
O2 K1 O2 66.04(14) 8_554 16 ?
Ir1 O1 Ir3 82.42(12) . . ?
Ir1 O1 K1 99.22(12) . 3 ?
Ir1 O1 K1 97.57(12) . . ?
Ir1 O1 K1 145.93(16) . 15 ?
Ir3 O1 K1 130.84(16) . 15 ?
Ir3 O1 K1 84.48(12) . 3 ?
Ir3 O1 K1 83.12(10) . . ?
K1 O1 K1 81.94(10) 15 . ?
K1 O1 K1 157.59(14) 3 . ?
K1 O1 K1 92.25(11) 15 3 ?
Ir2 O2 Ir3 81.87(12) . . ?
Ir2 O2 K1 92.07(11) . 16 ?
Ir2 O2 K1 101.17(14) . 6_455 ?
Ir2 O2 K1 168.07(16) . . ?
Ir3 O2 K1 125.49(15) . 16 ?
Ir3 O2 K1 153.50(16) . 6_455 ?
Ir3 O2 K1 86.91(12) . . ?
K1 O2 K1 87.09(10) 6_455 . ?
K1 O2 K1 97.78(11) . 16 ?
K1 O2 K1 80.92(9) 6_455 16 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ir1 Ir3 2.6459(4) . ?
Ir1 Ir3 2.6459(4) 10 ?
Ir1 K1 3.6676(13) . ?
Ir1 K1 3.6676(13) 10 ?
Ir1 K1 3.6676(13) 3 ?
Ir1 K1 3.6676(13) 12 ?
Ir1 O1 2.003(3) 11 ?
Ir1 O1 2.003(3) 2 ?
Ir1 O1 2.003(3) 12 ?
Ir1 O1 2.003(3) 3 ?
Ir1 O1 2.003(3) 10 ?
Ir1 O1 2.003(3) . ?
Ir2 Ir3 2.6249(4) 10_556 ?
Ir2 Ir3 2.6249(4) . ?
Ir2 K1 3.5886(12) 5 ?
Ir2 K1 3.5886(12) 16 ?
Ir2 K1 3.5886(12) 17_445 ?
Ir2 K1 3.5886(12) 4_445 ?
Ir2 O2 2.000(3) 11_556 ?
Ir2 O2 2.000(3) 2 ?
Ir2 O2 2.000(3) . ?
Ir2 O2 2.000(3) 3 ?
Ir2 O2 2.000(3) 10_556 ?
Ir2 O2 2.000(3) 12_556 ?
Ir3 K1 3.2622(12) . ?
Ir3 K1 3.2622(12) 2 ?
Ir3 K1 3.2622(12) 3 ?
Ir3 O1 2.013(3) . ?
Ir3 O1 2.013(3) 2 ?
Ir3 O1 2.013(3) 3 ?
Ir3 O2 2.007(3) . ?
Ir3 O2 2.007(3) 3 ?
Ir3 O2 2.007(3) 2 ?
K1 Ir2 3.5886(12) 7_554 ?
K1 K1 3.5925(12) 14_455 ?
K1 K1 3.6513(6) 8_554 ?
K1 K1 3.6514(6) 6_455 ?
K1 K1 3.5925(12) 15 ?
K1 O1 2.820(4) . ?
K1 O1 2.768(3) 2 ?
K1 O1 2.656(3) 14_455 ?
K1 O2 2.908(3) 16 ?
K1 O2 2.617(4) 8_554 ?
K1 O2 2.682(4) . ?
O1 K1 2.768(3) 3 ?
O1 K1 2.656(3) 15 ?
O2 K1 2.617(3) 6_455 ?
O2 K1 2.908(3) 16 ?
loop_
_twin_individual_id
_twin_individual_mass_fraction_refined
1 0.605(3)
2 0.395(3)
